Spreadsheet: 2356dacc-60fb-41cd-9075-114092c0521a
Sheet: 7. Titanium

 |  |  |  |  | MD-SLS; Part of SOP
M-spec |  | Linked standards |  | Material / Grade | Dimension limitation | Product | Certificate | Supplier NORSOK  M-650 qual. | Production process | Chemical composition |  |  |  | Yield & Tensile
 |  | NORSOK | Other |  |  |  |  |  |  | Cast / Ladle analysis |  | Product analysis |  | Minimum yield strength |  |  | [NAME] strength |  |  | Ratio | Elongation (minimum) |  |  | Bend test
 | rev. |  |  |  | m m |  |  |  |  | Element | Content % | Element | Content % | Dimention m m | KSI | MPa | Dimention m m | KSI | MPa | % | Dimension / Condition | % | Reduction of area | Dimensions | Report
M41202 | D | M630, T01, rev 4 | ASTM B 348 | Gr 2 |  | Bars & Billets | EN 10204 Type 3.1 or higher + manufacturer of the starting material of the finished product |  | Annealed condition if not the tensile properties in the referred standard can be achieved in as formed condition. | Nitrogen Carbon Hydrogen Iron Oxygen Total residuals* Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.03% max 0.08% max 0.015% max 0.30% max 0.25% max 0.4% Balance | Nitrogen Carbon Hydrogen Iron Oxygen Total residuals* Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.05% max 0.10% max 0.017% max 0.45% [NAME] 0.28% max 0.4% Balance |  | 40 | 275 |  | 50 | 345 |  |  | 20 | 30
M41202 | D | M630, T01, rev 4 | ASTM B 265 | Gr 2 |  | Strip. Sheet & Plate | EN 10204 Type 3.1 or higher + manufacturer of the starting material of the finished product | [NAME] qualified manufacturing procedure | Annealed condition if not the tensile properties in the referred standard can be achieved in as formed condition. | Nitrogen Carbon Hydrogen Iron Oxygen *Total residuals Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.03% max 0.08% max 0.015% max 0.30% max 0.25% max 0.4% Balance | Nitrogen Carbon Hydrogen Iron Oxygen Total residuals* Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.05% max 0.10% max 0.017% max 0.45% [NAME] 0.28% max 0.4% Balance |  | 40 - 65 | 275 - 345 |  | 50 | 345 |  |  | 20 | N/A
M41202 | D | M630, T01, rev 4 | ASTM B 861 | Gr 2 |  | Seamless pipes | EN 10204 Type 3.1 or higher + manufacturer of the starting material of the finished product | [NAME] qualified manufacturing procedure |  | Nitrogen Carbon Hydrogen Iron Oxygen *Total residuals Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.03% max 0.08% max 0.015% max 0.30% max 0.25% max 0.4% Balance | Nitrogen Carbon Hydrogen Iron Oxygen Total residuals* Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.05% max 0.10% max 0.017% max 0.45% [NAME] 0.28% max 0.4% Balance |  | 40 - 65 | 275 - 345 |  | 50 | 345 |  |  | 20 | N/A
M41202 | D | M630, T01, rev 4 | ASTM B 862 | Gr 2 |  | Welded pipes | EN 10204 Type 3.1 or higher + manufacturer of the starting material of the finished product | [NAME] qualified manufacturing procedure |  | Nitrogen Carbon Hydrogen Iron Oxygen *Total residuals Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.03% max 0.08% max 0.015% max 0.30% max 0.25% max 0.4% Balance | Nitrogen Carbon Hydrogen Iron Oxygen Total residuals* Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.05% max 0.10% max 0.017% max 0.45% [NAME] 0.28% max 0.4% Balance |  | 40 - 65 | 275 - 450 |  | 50 | 345
M41202 | D | M630, T01, rev 4 | ASTM B 338 | Gr 2 |  | Tubes | EN 10204 Type 3.1 or higher + manufacturer of the starting material of the finished product | [NAME] qualified manufacturing procedure |  | Nitrogen Carbon Hydrogen Iron Oxygen *Total residuals Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.03% max 0.08% max 0.015% max 0.30% max 0.25% max 0.4% Remainder | Nitrogen Carbon Hydrogen Iron Oxygen Total residuals* Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.05% max 0.10% max 0.017% max 0.45% [NAME] 0.28% max 0.4% Remainder |  | 40 - 65 | 275 - 450 |  | 50 | 345 |  |  | 20
M41202 | D | M630, T01, rev 4 | ASTM B 381 | F 2 |  | Forgings | EN 10204 Type 3.1 or higher + manufacturer of the starting material of the finished product | [NAME] qualified manufacturing procedure | Annealed condition if not the tensile properties in the referred standard can be achieved in as formed condition. | Nitrogen Carbon Hydrogen Iron Oxygen *Total residuals Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.03% max 0.08% max 0.015% max 0.30% max 0.25% max 0.4% Balance | Nitrogen Carbon Hydrogen Iron Oxygen Total residuals* Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.05% max 0.10% max 0.017% max 0.45% [NAME] 0.28% max 0.4% Balance |  | 40 | 275 |  | 50 | 345 |  |  | 20 | 30
M41202 | D | M630, T01, rev 4 | ASTM B 363 WPT2/WPT2W | Gr 2 |  | Wrought fittings | EN 10204 Type 3.1 or higher + manufacturer of the starting material of the finished product | [NAME] qualified manufacturing procedure | Annealed condition if not the tensile properties in the referred standard can be achieved in                                                                                                                                                                                                                                               as formed condition. | Same requirements as for all raw products listed abow dependent on the rawmaterial for the fitting, either it is bar, pipe, plate etc.
M41202 | C | M630, T01, rev 4 | ASTM B 348 | Gr 2 |  | Bars & Billets | EN 10204 Type 3.1 or higher + manufacturer of the starting material of the finished product |  | Annealed condition to fulfil tensile properties | Nitrogen Carbon Hydrogen Iron Oxygen Total residuals* Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.03% max 0.08% max 0.015% max 0.30% max 0.25% max 0.4% Remainder | Nitrogen Carbon Hydrogen Iron Oxygen Total residuals* Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.05% max 0.10% max 0.017% max 0.45% [NAME] 0.28% max 0.4% Remainder |  | 40 | 275 |  | 50 | 345 |  |  | 20 | 30
M41202 | C | M630, T01, rev 4 | ASTM B 265 | Gr 2 |  | Strip. Sheet & Plate | EN 10204 Type 3.1 or higher + manufacturer of the starting material of the finished product | [NAME] qualified manufacturing procedure | Annealed condition to fulfil tensile properties | Nitrogen Carbon Hydrogen Iron Oxygen *Total residuals Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.03% max 0.08% max 0.015% max 0.30% max 0.25% max 0.4% Remainder | Nitrogen Carbon Hydrogen Iron Oxygen Total residuals* Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.05% max 0.10% max 0.017% max 0.45% [NAME] 0.28% max 0.4% Remainder |  | 40 - 65 | 275 - 450 |  | 50 | 345 |  |  | 20 |  | t<4.75mm | acceptable
M41202 | C | M630, T01, rev 4 | ASTM B 861 | Gr 2 |  | Seamless pipes | EN 10204 Type 3.1 or higher + manufacturer of the starting material of the finished product | [NAME] qualified manufacturing procedure |  | Nitrogen Carbon Hydrogen Iron Oxygen *Total residuals Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.03% max 0.08% max 0.015% max 0.30% max 0.25% max 0.4% Remainder | Nitrogen Carbon Hydrogen Iron Oxygen Total residuals* Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.05% max 0.10% max 0.017% max 0.45% [NAME] 0.28% max 0.4% Remainder |  | 40 - 65 | 275 - 450 |  | 50 | 345 |  |  | 20 |  | dia<51mm | acceptable
M41202 | C | M630, T01, rev 4 | ASTM B 862 | Gr 2 |  | Welded pipes | EN 10204 Type 3.1 or higher + manufacturer of the starting material of the finished product | [NAME] qualified manufacturing procedure |  | Nitrogen Carbon Hydrogen Iron Oxygen *Total residuals Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.03% max 0.08% max 0.015% max 0.30% max 0.25% max 0.4% Remainder | Nitrogen Carbon Hydrogen Iron Oxygen Total residuals* Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.05% max 0.10% max 0.017% max 0.45% [NAME] 0.28% max 0.4% Remainder |  | 40 - 65 | 275 - 450 |  | 50 | 345
M41202 | C | M630, T01, rev 4 | ASTM B 338 | Gr 2 |  | Tubes | EN 10204 Type 3.1 or higher + manufacturer of the starting material of the finished product | [NAME] qualified manufacturing procedure | Annealed condition to fulfil tensile properties | Nitrogen Carbon Hydrogen Iron Oxygen *Total residuals Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.03% max 0.08% max 0.015% max 0.30% max 0.25% max 0.4% Remainder | Nitrogen Carbon Hydrogen Iron Oxygen Total residuals* Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.05% max 0.10% max 0.017% max 0.45% [NAME] 0.28% max 0.4% Remainder |  | 40 - 65 | 275 - 450 |  | 50 | 345 |  |  | 20
M41202 | C | M630, T01, rev 4 | ASTM B 381 | Gr 2 |  | Forgings | EN 10204 Type 3.1 or higher + manufacturer of the starting material of the finished product | [NAME] qualified manufacturing procedure | Annealed condition to fulfil tensile properties | Nitrogen Carbon Hydrogen Iron Oxygen *Total residuals Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.03% max 0.08% max 0.015% max 0.30% max 0.25% max 0.4% Remainder | Nitrogen Carbon Hydrogen Iron Oxygen Total residuals* Titanium  *Total residuals content is not required for routine acceptance. | [NAME] 0.05% max 0.10% max 0.017% max 0.45% [NAME] 0.28% max 0.4% Remainder |  | 40 | 275 |  | 50 | 345 |  |  | 20 | 30
M41202 | C | M630, T01, rev 4 | ASTM B 363 WPT2/WPT2W | Gr 2 |  | Wrought fittings | EN 10204 Type 3.1 or higher + manufacturer of the starting material of the finished product | [NAME] qualified manufacturing procedure | Annealed condition to fulfil tensile properties | Same requirements as for all raw products listed abow dependent on the rawmaterial for the fitting, either it is bar, pipe, plate etc.